#------------------------------------------------------------------------------
#$Date: 2016-02-20 18:35:30 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176787 $
#$URL: svn://www.crystallography.net/cod/cif/2/21/46/2214637.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2214637
loop_
_publ_author_name
'Xia, Ming-Jun'
'Li, R. K.'
_publ_section_title
;
 A new quaternary rare earth borate, CsLi₂Gd₄(BO₃)₅
;
_journal_coeditor_code           FI2036
_journal_issue                   8
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i173
_journal_page_last               i173
_journal_paper_doi               10.1107/S1600536807036586
_journal_volume                  63
_journal_year                    2007
_chemical_formula_iupac          'Cs Li2 Gd4 (B O3)5'
_chemical_formula_moiety         'B5 Gd4 O15 , Cs , 2Li'
_chemical_formula_sum            'B5 Cs Gd4 Li2 O15'
_chemical_formula_weight         1069.84
_chemical_name_common
'caesium dilithium tetragadolinium pentaborate'
_chemical_name_systematic
;
caesium dilithium tetragadolinium pentaborate
;
_space_group_IT_number           13
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yac'
_symmetry_space_group_name_H-M   'P 1 2/n 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL97
_cell_angle_alpha                90.00
_cell_angle_beta                 105.250(16)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   10.644(2)
_cell_length_b                   6.4661(15)
_cell_length_c                   20.093(4)
_cell_measurement_reflns_used    23
_cell_measurement_temperature    295(2)
_cell_measurement_theta_max      11.7
_cell_measurement_theta_min      6.5
_cell_volume                     1334.2(5)
_computing_cell_refinement       XSCANS
_computing_data_collection       'XSCANS (Bruker, 1997)'
_computing_data_reduction        'SHELXTL (Bruker, 1997)'
_computing_molecular_graphics    'ORTEP-3 for Windows (Farrugia, 1997)'
_computing_publication_material  'publCIF (Version 1.0c; Westrip, 2007)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      295(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0604
_diffrn_reflns_av_sigmaI/netI    0.0582
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            7381
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         27.50
_diffrn_reflns_theta_min         1.98
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 97
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    22.396
_exptl_absorpt_correction_T_max  0.1670
_exptl_absorpt_correction_T_min  0.0418
_exptl_absorpt_correction_type   psi-scan
_exptl_absorpt_process_details   '(North et al.,  1968)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    5.326
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1848
_exptl_crystal_size_max          0.16
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.08
_refine_diff_density_max         4.052
_refine_diff_density_min         -2.807
_refine_ls_extinction_coef       0.0133(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL97 (Sheldrick, 1997)'
_refine_ls_goodness_of_fit_ref   1.106
_refine_ls_matrix_type           full
_refine_ls_number_parameters     248
_refine_ls_number_reflns         3068
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.106
_refine_ls_R_factor_all          0.0465
_refine_ls_R_factor_gt           0.0443
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w = 1/[σ²(Fo²)+(0.0690P)²+1.5286P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1041
_refine_ls_wR_factor_ref         0.1081
_reflns_number_gt                2829
_reflns_number_total             3068
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            fi2036.cif
_cod_data_source_block           I
_cod_original_cell_volume        1334.3(5)
_cod_original_sg_symbol_H-M      'P 2/n'
_cod_database_code               2214637
_cod_database_fobs_code          2214637
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, y, -z+1/2'
'-x, -y, -z'
'x-1/2, -y, z-1/2'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
Gd Gd1 0.45528(3) 0.34144(6) 0.649931(16) 0.01704(15) Uani d . 1
Gd Gd2 0.2500 0.59641(9) 0.7500 0.02208(16) Uani d S 1
Gd Gd3 0.7500 0.59044(8) 0.7500 0.01776(16) Uani d S 1
Gd Gd4 0.35686(3) 0.64428(6) 0.946524(18) 0.01724(14) Uani d . 1
Gd Gd5 0.84343(3) 0.64848(6) 0.953592(16) 0.01731(15) Uani d . 1
Cs Cs1 0.55501(4) 0.09547(9) 0.85836(2) 0.02535(16) Uani d . 1
B B1 0.4515(6) 0.7837(16) 0.6497(4) 0.0190(16) Uani d . 1
B B2 0.2500 0.1655(18) 0.7500 0.020(2) Uani d S 1
B B3 0.7500 0.1618(19) 0.7500 0.023(3) Uani d S 1
B B4 0.3429(7) 0.1954(19) 0.9500(4) 0.0238(19) Uani d . 1
B B5 0.8570(8) 0.2030(17) 0.9562(4) 0.0216(17) Uani d . 1
B B6 0.5418(7) 0.5930(13) 0.8231(4) 0.0200(15) Uani d . 1
Li Li1 0.6372(11) 0.978(2) 0.6532(7) 0.027(3) Uani d . 1
Li Li2 0.2786(11) 0.987(2) 0.6582(6) 0.022(2) Uani d . 1
O O1 0.4590(4) 0.9903(9) 0.6603(3) 0.0231(11) Uani d . 1
O O2 0.3386(5) 0.6737(8) 0.6485(3) 0.0198(11) Uani d . 1
O O3 0.5582(5) 0.6740(8) 0.6405(3) 0.0189(10) Uani d . 1
O O4 0.2500 -0.0436(13) 0.7500 0.0252(17) Uani d S 1
O O5 0.2777(4) 0.2764(8) 0.6974(2) 0.0207(10) Uani d . 1
O O6 0.7500 -0.0510(13) 0.7500 0.0226(17) Uani d S 1
O O7 0.8179(4) 0.2672(9) 0.8072(2) 0.0206(10) Uani d . 1
O O8 0.3404(4) -0.0048(9) 0.9297(3) 0.0190(10) Uani d . 1
O O9 0.4550(4) 0.3091(9) 0.9728(3) 0.0237(11) Uani d . 1
O O10 0.2302(4) 0.3107(8) 0.9469(3) 0.0202(10) Uani d . 1
O O11 0.8424(5) -0.0004(10) 0.9383(3) 0.0203(10) Uani d . 1
O O12 0.9664(5) 0.3213(8) 0.9531(3) 0.0191(10) Uani d . 1
O O13 0.7622(4) 0.3197(8) 0.9754(3) 0.0220(10) Uani d . 1
O O14 0.5248(5) 0.4966(10) 0.7606(3) 0.0265(11) Uani d . 1
O O15 0.6689(4) 0.6496(9) 0.8568(3) 0.0219(11) Uani d . 1
O O16 0.4352(5) 0.6364(9) 0.8473(3) 0.0233(11) Uani d . 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O1 Gd1 O5 1_545 . 77.44(17)
O1 Gd1 O14 1_545 . 110.0(2)
O5 Gd1 O14 . . 77.49(17)
O1 Gd1 O10 1_545 2_556 88.99(18)
O5 Gd1 O10 . 2_556 74.75(16)
O14 Gd1 O10 . 2_556 141.81(18)
O1 Gd1 O7 1_545 2_656 77.01(18)
O5 Gd1 O7 . 2_656 131.07(17)
O14 Gd1 O7 . 2_656 73.17(17)
O10 Gd1 O7 2_556 2_656 144.84(17)
O1 Gd1 O12 1_545 2_656 91.33(18)
O5 Gd1 O12 . 2_656 145.34(17)
O14 Gd1 O12 . 2_656 136.74(18)
O10 Gd1 O12 2_556 2_656 72.34(17)
O7 Gd1 O12 2_656 2_656 75.88(16)
O1 Gd1 O3 1_545 . 152.44(16)
O5 Gd1 O3 . . 127.53(17)
O14 Gd1 O3 . . 70.40(19)
O10 Gd1 O3 2_556 . 107.56(17)
O7 Gd1 O3 2_656 . 76.93(18)
O12 Gd1 O3 2_656 . 73.74(17)
O1 Gd1 O2 1_545 . 149.44(16)
O5 Gd1 O2 . . 73.01(17)
O14 Gd1 O2 . . 71.09(19)
O10 Gd1 O2 2_556 . 76.03(18)
O7 Gd1 O2 2_656 . 129.38(17)
O12 Gd1 O2 2_656 . 108.66(17)
O3 Gd1 O2 . . 57.97(17)
O1 Gd1 B1 1_545 . 174.87(19)
O5 Gd1 B1 . . 99.54(19)
O14 Gd1 B1 . . 65.1(2)
O10 Gd1 B1 2_556 . 94.24(19)
O7 Gd1 B1 2_656 . 102.36(19)
O12 Gd1 B1 2_656 . 93.45(19)
O3 Gd1 B1 . . 29.10(17)
O2 Gd1 B1 . . 29.11(17)
O1 Gd1 Li2 1_545 1_545 39.5(3)
O5 Gd1 Li2 . 1_545 42.5(3)
O14 Gd1 Li2 . 1_545 108.5(3)
O10 Gd1 Li2 2_556 1_545 65.5(3)
O7 Gd1 Li2 2_656 1_545 114.5(3)
O12 Gd1 Li2 2_656 1_545 111.5(3)
O3 Gd1 Li2 . 1_545 168.0(3)
O2 Gd1 Li2 . 1_545 110.1(3)
B1 Gd1 Li2 . 1_545 139.1(3)
O1 Gd1 Li1 1_545 1_545 39.8(3)
O5 Gd1 Li1 . 1_545 115.2(3)
O14 Gd1 Li1 . 1_545 105.5(3)
O10 Gd1 Li1 2_556 1_545 109.9(3)
O7 Gd1 Li1 2_656 1_545 42.1(3)
O12 Gd1 Li1 2_656 1_545 67.5(3)
O3 Gd1 Li1 . 1_545 112.7(3)
O2 Gd1 Li1 . 1_545 170.6(3)
B1 Gd1 Li1 . 1_545 141.5(3)
Li2 Gd1 Li1 1_545 1_545 79.2(4)
O1 Gd1 Gd3 1_545 . 113.56(12)
O5 Gd1 Gd3 . . 121.42(12)
O14 Gd1 Gd3 . . 44.10(12)
O10 Gd1 Gd3 2_556 . 153.86(13)
O7 Gd1 Gd3 2_656 . 40.95(13)
O12 Gd1 Gd3 2_656 . 93.18(12)
O3 Gd1 Gd3 . . 46.54(11)
O2 Gd1 Gd3 . . 88.82(12)
B1 Gd1 Gd3 . . 64.33(13)
Li2 Gd1 Gd3 1_545 . 140.6(2)
Li1 Gd1 Gd3 1_545 . 82.9(2)
O4 Gd2 O5 1_565 . 150.52(11)
O4 Gd2 O5 1_565 2_556 150.52(11)
O5 Gd2 O5 . 2_556 59.0(2)
O4 Gd2 O16 1_565 2_556 83.80(14)
O5 Gd2 O16 . 2_556 84.42(18)
O5 Gd2 O16 2_556 2_556 106.56(18)
O4 Gd2 O16 1_565 . 83.80(14)
O5 Gd2 O16 . . 106.56(17)
O5 Gd2 O16 2_556 . 84.42(18)
O16 Gd2 O16 2_556 . 167.6(3)
O4 Gd2 O2 1_565 . 78.52(12)
O5 Gd2 O2 . . 72.26(16)
O5 Gd2 O2 2_556 . 130.64(17)
O16 Gd2 O2 2_556 . 73.76(17)
O16 Gd2 O2 . . 103.69(17)
O4 Gd2 O2 1_565 2_556 78.52(12)
O5 Gd2 O2 . 2_556 130.64(17)
O5 Gd2 O2 2_556 2_556 72.26(16)
O16 Gd2 O2 2_556 2_556 103.69(17)
O16 Gd2 O2 . 2_556 73.76(17)
O2 Gd2 O2 . 2_556 157.0(2)
O4 Gd2 B2 1_565 . 180.000(4)
O5 Gd2 B2 . . 29.48(11)
O5 Gd2 B2 2_556 . 29.48(11)
O16 Gd2 B2 2_556 . 96.20(14)
O16 Gd2 B2 . . 96.20(14)
O2 Gd2 B2 . . 101.48(12)
O2 Gd2 B2 2_556 . 101.48(12)
O4 Gd2 O14 1_565 2_556 102.64(13)
O5 Gd2 O14 . 2_556 90.81(16)
O5 Gd2 O14 2_556 2_556 66.72(16)
O16 Gd2 O14 2_556 2_556 51.50(16)
O16 Gd2 O14 . 2_556 132.05(16)
O2 Gd2 O14 . 2_556 124.22(15)
O2 Gd2 O14 2_556 2_556 61.62(15)
B2 Gd2 O14 . 2_556 77.36(13)
O4 Gd2 O14 1_565 . 102.64(13)
O5 Gd2 O14 . . 66.72(16)
O5 Gd2 O14 2_556 . 90.81(16)
O16 Gd2 O14 2_556 . 132.05(16)
O16 Gd2 O14 . . 51.50(16)
O2 Gd2 O14 . . 61.62(15)
O2 Gd2 O14 2_556 . 124.22(15)
B2 Gd2 O14 . . 77.36(13)
O14 Gd2 O14 2_556 . 154.7(3)
O4 Gd2 B6 1_565 2_556 90.41(16)
O5 Gd2 B6 . 2_556 90.52(19)
O5 Gd2 B6 2_556 2_556 88.76(19)
O16 Gd2 B6 2_556 2_556 25.60(19)
O16 Gd2 B6 . 2_556 154.60(19)
O2 Gd2 B6 . 2_556 99.31(18)
O2 Gd2 B6 2_556 2_556 80.86(18)
B2 Gd2 B6 . 2_556 89.59(16)
O14 Gd2 B6 2_556 2_556 26.27(17)
O14 Gd2 B6 . 2_556 153.33(18)
O4 Gd2 B6 1_565 . 90.41(16)
O5 Gd2 B6 . . 88.76(19)
O5 Gd2 B6 2_556 . 90.52(19)
O16 Gd2 B6 2_556 . 154.60(19)
O16 Gd2 B6 . . 25.60(19)
O2 Gd2 B6 . . 80.86(18)
O2 Gd2 B6 2_556 . 99.31(18)
B2 Gd2 B6 . . 89.59(16)
O14 Gd2 B6 2_556 . 153.33(18)
O14 Gd2 B6 . . 26.27(17)
B6 Gd2 B6 2_556 . 179.2(3)
O6 Gd3 O7 1_565 . 150.44(11)
O6 Gd3 O7 1_565 2_656 150.44(11)
O7 Gd3 O7 . 2_656 59.1(2)
O6 Gd3 O14 1_565 . 103.85(15)
O7 Gd3 O14 . . 85.64(17)
O7 Gd3 O14 2_656 . 70.10(17)
O6 Gd3 O14 1_565 2_656 103.85(15)
O7 Gd3 O14 . 2_656 70.10(17)
O7 Gd3 O14 2_656 2_656 85.64(17)
O14 Gd3 O14 . 2_656 152.3(3)
O6 Gd3 O15 1_565 2_656 81.35(13)
O7 Gd3 O15 . 2_656 114.08(16)
O7 Gd3 O15 2_656 2_656 81.59(17)
O14 Gd3 O15 . 2_656 130.14(16)
O14 Gd3 O15 2_656 2_656 55.07(16)
O6 Gd3 O15 1_565 . 81.34(13)
O7 Gd3 O15 . . 81.59(17)
O7 Gd3 O15 2_656 . 114.08(17)
O14 Gd3 O15 . . 55.07(16)
O14 Gd3 O15 2_656 . 130.14(16)
O15 Gd3 O15 2_656 . 162.7(3)
O6 Gd3 O3 1_565 2_656 78.17(11)
O7 Gd3 O3 . 2_656 73.11(16)
O7 Gd3 O3 2_656 2_656 130.34(16)
O14 Gd3 O3 . 2_656 121.44(16)
O14 Gd3 O3 2_656 2_656 64.95(16)
O15 Gd3 O3 2_656 2_656 108.25(16)
O15 Gd3 O3 . 2_656 67.98(16)
O6 Gd3 O3 1_565 . 78.17(11)
O7 Gd3 O3 . . 130.34(16)
O7 Gd3 O3 2_656 . 73.11(16)
O14 Gd3 O3 . . 64.95(16)
O14 Gd3 O3 2_656 . 121.44(16)
O15 Gd3 O3 2_656 . 67.98(16)
O15 Gd3 O3 . . 108.25(16)
O3 Gd3 O3 2_656 . 156.3(2)
O6 Gd3 B3 1_565 . 180.000(3)
O7 Gd3 B3 . . 29.56(11)
O7 Gd3 B3 2_656 . 29.56(11)
O14 Gd3 B3 . . 76.15(15)
O14 Gd3 B3 2_656 . 76.15(15)
O15 Gd3 B3 2_656 . 98.65(13)
O15 Gd3 B3 . . 98.66(13)
O3 Gd3 B3 2_656 . 101.83(11)
O3 Gd3 B3 . . 101.83(11)
O6 Gd3 B6 1_565 . 89.68(16)
O7 Gd3 B6 . . 86.45(19)
O7 Gd3 B6 2_656 . 94.11(19)
O14 Gd3 B6 . . 27.51(18)
O14 Gd3 B6 2_656 . 152.8(2)
O15 Gd3 B6 2_656 . 151.79(18)
O15 Gd3 B6 . . 28.00(18)
O3 Gd3 B6 2_656 . 95.82(18)
O3 Gd3 B6 . . 84.05(19)
B3 Gd3 B6 . . 90.32(17)
O6 Gd3 B6 1_565 2_656 89.68(17)
O7 Gd3 B6 . 2_656 94.11(19)
O7 Gd3 B6 2_656 2_656 86.45(19)
O14 Gd3 B6 . 2_656 152.8(2)
O14 Gd3 B6 2_656 2_656 27.51(18)
O15 Gd3 B6 2_656 2_656 28.00(18)
O15 Gd3 B6 . 2_656 151.79(19)
O3 Gd3 B6 2_656 2_656 84.05(19)
O3 Gd3 B6 . 2_656 95.82(18)
B3 Gd3 B6 . 2_656 90.32(16)
B6 Gd3 B6 . 2_656 179.4(3)
O9 Gd4 O13 3_667 3_667 92.37(18)
O9 Gd4 O8 3_667 1_565 89.57(18)
O13 Gd4 O8 3_667 1_565 88.01(18)
O9 Gd4 O16 3_667 . 99.64(19)
O13 Gd4 O16 3_667 . 166.45(18)
O8 Gd4 O16 1_565 . 85.83(19)
O9 Gd4 O9 3_667 . 73.0(2)
O13 Gd4 O9 3_667 . 103.30(18)
O8 Gd4 O9 1_565 . 159.41(17)
O16 Gd4 O9 . . 86.33(19)
O9 Gd4 O2 3_667 2_556 166.9(2)
O13 Gd4 O2 3_667 2_556 90.96(17)
O8 Gd4 O2 1_565 2_556 77.92(17)
O16 Gd4 O2 . 2_556 75.95(18)
O9 Gd4 O2 . 2_556 118.38(17)
O9 Gd4 O10 3_667 . 119.01(18)
O13 Gd4 O10 3_667 . 72.09(17)
O8 Gd4 O10 1_565 . 144.98(16)
O16 Gd4 O10 . . 106.88(18)
O9 Gd4 O10 . . 55.60(16)
O2 Gd4 O10 2_556 . 74.02(17)
O9 Gd4 B4 3_667 . 99.1(2)
O13 Gd4 B4 3_667 . 92.5(2)
O8 Gd4 B4 1_565 . 171.27(19)
O16 Gd4 B4 . . 91.8(2)
O9 Gd4 B4 . . 27.96(18)
O2 Gd4 B4 2_556 . 93.36(19)
O10 Gd4 B4 . . 28.77(18)
O9 Gd4 Li2 3_667 2_556 123.9(3)
O13 Gd4 Li2 3_667 2_556 98.6(2)
O8 Gd4 Li2 1_565 2_556 36.7(3)
O16 Gd4 Li2 . 2_556 69.5(3)
O9 Gd4 Li2 . 2_556 151.8(3)
O2 Gd4 Li2 2_556 2_556 43.1(3)
O10 Gd4 Li2 . 2_556 116.8(3)
B4 Gd4 Li2 . 2_556 134.8(3)
O9 Gd4 Gd4 3_667 3_667 38.01(14)
O13 Gd4 Gd4 3_667 3_667 99.95(13)
O8 Gd4 Gd4 1_565 3_667 126.73(12)
O16 Gd4 Gd4 . 3_667 93.40(13)
O9 Gd4 Gd4 . 3_667 35.04(12)
O2 Gd4 Gd4 2_556 3_667 152.96(13)
O10 Gd4 Gd4 . 3_667 85.84(11)
B4 Gd4 Gd4 . 3_667 61.74(15)
Li2 Gd4 Gd4 2_556 3_667 154.4(2)
O9 Gd4 Gd5 3_667 3_667 101.76(14)
O13 Gd4 Gd5 3_667 3_667 36.24(13)
O8 Gd4 Gd5 1_565 3_667 122.64(13)
O16 Gd4 Gd5 . 3_667 144.10(14)
O9 Gd4 Gd5 . 3_667 72.93(12)
O2 Gd4 Gd5 2_556 3_667 88.34(12)
O10 Gd4 Gd5 . 3_667 37.24(11)
B4 Gd4 Gd5 . 3_667 56.64(16)
Li2 Gd4 Gd5 2_556 3_667 119.0(2)
Gd4 Gd4 Gd5 3_667 3_667 86.18(2)
O9 Gd4 Gd2 3_667 . 136.44(13)
O13 Gd4 Gd2 3_667 . 130.73(13)
O8 Gd4 Gd2 1_565 . 86.43(12)
O16 Gd4 Gd2 . . 36.82(13)
O9 Gd4 Gd2 . . 98.50(13)
O2 Gd4 Gd2 2_556 . 40.10(12)
O10 Gd4 Gd2 . . 85.46(11)
B4 Gd4 Gd2 . . 86.62(15)
Li2 Gd4 Gd2 2_556 . 53.4(2)
Gd4 Gd4 Gd2 3_667 . 122.01(2)
Gd5 Gd4 Gd2 3_667 . 116.732(17)
O11 Gd5 O15 1_565 . 84.81(19)
O11 Gd5 O10 1_565 3_667 90.68(19)
O15 Gd5 O10 . 3_667 110.01(17)
O11 Gd5 O12 1_565 3_767 89.85(18)
O15 Gd5 O12 . 3_767 173.27(18)
O10 Gd5 O12 3_667 3_767 74.05(18)
O11 Gd5 O13 1_565 . 157.13(17)
O15 Gd5 O13 . . 84.69(18)
O10 Gd5 O13 3_667 . 74.01(19)
O12 Gd5 O13 3_767 . 101.74(17)
O11 Gd5 O3 1_565 2_656 79.26(19)
O15 Gd5 O3 . 2_656 75.92(18)
O10 Gd5 O3 3_667 2_656 167.96(19)
O12 Gd5 O3 3_767 2_656 99.10(17)
O13 Gd5 O3 . 2_656 117.54(17)
O11 Gd5 O12 1_565 . 145.68(17)
O15 Gd5 O12 . . 107.87(18)
O10 Gd5 O12 3_667 . 113.12(17)
O12 Gd5 O12 3_767 . 74.52(19)
O13 Gd5 O12 . . 57.18(16)
O3 Gd5 O12 2_656 . 73.51(17)
O11 Gd5 B5 1_565 . 172.2(2)
O15 Gd5 B5 . . 92.5(2)
O10 Gd5 B5 3_667 . 97.1(2)
O12 Gd5 B5 3_767 . 92.3(2)
O13 Gd5 B5 . . 28.69(19)
O3 Gd5 B5 2_656 . 93.0(2)
O12 Gd5 B5 . . 29.22(19)
O11 Gd5 Li1 1_565 2_656 38.4(3)
O15 Gd5 Li1 . 2_656 66.2(3)
O10 Gd5 Li1 3_667 2_656 128.0(3)
O12 Gd5 Li1 3_767 2_656 107.1(3)
O13 Gd5 Li1 . 2_656 147.6(3)
O3 Gd5 Li1 2_656 2_656 43.7(3)
O12 Gd5 Li1 . 2_656 117.1(3)
B5 Gd5 Li1 . 2_656 134.0(3)
O11 Gd5 Gd4 1_565 3_667 125.57(13)
O15 Gd5 Gd4 . 3_667 90.44(13)
O10 Gd5 Gd4 3_667 3_667 41.03(13)
O12 Gd5 Gd4 3_767 3_667 95.99(12)
O13 Gd5 Gd4 . 3_667 34.40(12)
O3 Gd5 Gd4 2_656 3_667 150.98(12)
O12 Gd5 Gd4 . 3_667 86.96(12)
B5 Gd5 Gd4 . 3_667 61.61(16)
Li1 Gd5 Gd4 2_656 3_667 150.0(2)
O11 Gd5 Gd1 1_565 4_666 96.38(14)
O15 Gd5 Gd1 . 4_666 146.63(13)
O10 Gd5 Gd1 3_667 4_666 36.80(12)
O12 Gd5 Gd1 3_767 4_666 38.09(12)
O13 Gd5 Gd1 . 4_666 81.61(13)
O3 Gd5 Gd1 2_656 4_666 137.19(12)
O12 Gd5 Gd1 . 4_666 89.83(12)
B5 Gd5 Gd1 . 4_666 89.87(15)
Li1 Gd5 Gd1 2_656 4_666 130.7(3)
Gd4 Gd5 Gd1 3_667 4_666 61.771(15)
O11 Gd5 Gd5 1_565 3_767 121.94(13)
O15 Gd5 Gd5 . 3_767 143.78(13)
O10 Gd5 Gd5 3_667 3_767 94.80(12)
O12 Gd5 Gd5 3_767 3_767 38.26(13)
O13 Gd5 Gd5 . 3_767 77.09(12)
O3 Gd5 Gd5 2_656 3_767 85.11(12)
O12 Gd5 Gd5 . 3_767 36.27(11)
B5 Gd5 Gd5 . 3_767 57.56(16)
Li1 Gd5 Gd5 2_656 3_767 118.3(2)
Gd4 Gd5 Gd5 3_667 3_767 91.72(2)
Gd1 Gd5 Gd5 4_666 3_767 60.984(16)
O8 Cs1 O9 . . 45.95(14)
O8 Cs1 O11 . . 117.84(15)
O9 Cs1 O11 . . 100.84(14)
O8 Cs1 O13 . . 102.18(13)
O9 Cs1 O13 . . 63.08(13)
O11 Cs1 O13 . . 45.78(14)
O8 Cs1 O15 . 1_545 98.52(14)
O9 Cs1 O15 . 1_545 128.84(14)
O11 Cs1 O15 . 1_545 59.50(14)
O13 Cs1 O15 . 1_545 103.66(13)
O8 Cs1 O16 . 1_545 60.46(14)
O9 Cs1 O16 . 1_545 104.80(14)
O11 Cs1 O16 . 1_545 99.76(15)
O13 Cs1 O16 . 1_545 131.98(13)
O15 Cs1 O16 1_545 1_545 45.32(14)
O8 Cs1 O14 . . 119.24(13)
O9 Cs1 O14 . . 95.46(14)
O11 Cs1 O14 . . 113.65(14)
O13 Cs1 O14 . . 91.31(14)
O15 Cs1 O14 1_545 . 135.44(14)
O16 Cs1 O14 1_545 . 136.69(14)
O8 Cs1 B6 . . 108.20(17)
O9 Cs1 B6 . . 73.76(17)
O11 Cs1 B6 . . 106.59(17)
O13 Cs1 B6 . . 71.94(16)
O15 Cs1 B6 1_545 . 153.27(16)
O16 Cs1 B6 1_545 . 153.43(16)
O14 Cs1 B6 . . 24.31(16)
O8 Cs1 B6 . 1_545 84.15(16)
O9 Cs1 B6 . 1_545 126.20(17)
O11 Cs1 B6 . 1_545 84.04(17)
O13 Cs1 B6 . 1_545 126.61(16)
O15 Cs1 B6 1_545 1_545 24.72(15)
O16 Cs1 B6 1_545 1_545 24.23(15)
O14 Cs1 B6 . 1_545 131.79(18)
B6 Cs1 B6 . 1_545 156.1(3)
O8 Cs1 B4 . . 24.0(2)
O9 Cs1 B4 . . 24.33(19)
O11 Cs1 B4 . . 117.98(16)
O13 Cs1 B4 . . 86.60(18)
O15 Cs1 B4 1_545 . 120.3(2)
O16 Cs1 B4 1_545 . 84.4(2)
O14 Cs1 B4 . . 102.0(2)
B6 Cs1 B4 . . 86.1(2)
B6 Cs1 B4 1_545 . 108.1(2)
O8 Cs1 B5 . . 118.94(16)
O9 Cs1 B5 . . 86.34(17)
O11 Cs1 B5 . . 23.8(2)
O13 Cs1 B5 . . 24.39(17)
O15 Cs1 B5 1_545 . 83.3(2)
O16 Cs1 B5 1_545 . 122.1(2)
O14 Cs1 B5 . . 96.7(2)
B6 Cs1 B5 . . 84.5(2)
B6 Cs1 B5 1_545 . 107.9(2)
B4 Cs1 B5 . . 108.6(2)
O8 Cs1 B3 . . 168.12(13)
O9 Cs1 B3 . . 143.5(2)
O11 Cs1 B3 . . 71.00(12)
O13 Cs1 B3 . . 89.69(14)
O15 Cs1 B3 1_545 . 78.9(2)
O16 Cs1 B3 1_545 . 111.7(2)
O14 Cs1 B3 . . 59.2(2)
B6 Cs1 B3 . . 74.8(3)
B6 Cs1 B3 1_545 . 89.2(2)
B4 Cs1 B3 . . 160.8(3)
B5 Cs1 B3 . . 72.48(14)
O1 B1 O2 . . 121.5(6)
O1 B1 O3 . . 120.6(7)
O2 B1 O3 . . 117.9(8)
O1 B1 Li2 . . 56.0(5)
O2 B1 Li2 . . 65.7(5)
O3 B1 Li2 . . 174.9(7)
O1 B1 Li1 . . 56.4(5)
O2 B1 Li1 . . 177.9(7)
O3 B1 Li1 . . 64.2(5)
Li2 B1 Li1 . . 112.2(7)
O1 B1 Gd1 . . 171.0(5)
O2 B1 Gd1 . . 60.0(4)
O3 B1 Gd1 . . 58.6(4)
Li2 B1 Gd1 . . 125.5(4)
Li1 B1 Gd1 . . 121.9(5)
O4 B2 O5 . 2_556 121.5(5)
O4 B2 O5 . . 121.5(5)
O5 B2 O5 2_556 . 117.0(9)
O4 B2 Li2 . 2_546 59.3(4)
O5 B2 Li2 2_556 2_546 62.4(4)
O5 B2 Li2 . 2_546 175.3(4)
O4 B2 Li2 . 1_545 59.3(4)
O5 B2 Li2 2_556 1_545 175.3(4)
O5 B2 Li2 . 1_545 62.4(4)
Li2 B2 Li2 2_546 1_545 118.6(8)
O4 B2 Gd2 . . 180.000(3)
O5 B2 Gd2 2_556 . 58.5(5)
O5 B2 Gd2 . . 58.5(5)
Li2 B2 Gd2 2_546 . 120.7(4)
Li2 B2 Gd2 1_545 . 120.7(4)
O4 B2 Cs1 . . 82.41(19)
O5 B2 Cs1 2_556 . 86.51(19)
O5 B2 Cs1 . . 101.5(2)
Li2 B2 Cs1 2_546 . 73.9(3)
Li2 B2 Cs1 1_545 . 98.2(3)
Gd2 B2 Cs1 . . 97.59(19)
O4 B2 Cs1 . 2_556 82.41(19)
O5 B2 Cs1 2_556 2_556 101.5(2)
O5 B2 Cs1 . 2_556 86.51(19)
Li2 B2 Cs1 2_546 2_556 98.2(3)
Li2 B2 Cs1 1_545 2_556 73.9(3)
Gd2 B2 Cs1 . 2_556 97.59(19)
Cs1 B2 Cs1 . 2_556 164.8(4)
O7 B3 O7 2_656 . 120.2(10)
O7 B3 O6 2_656 . 119.9(5)
O7 B3 O6 . . 119.9(5)
O7 B3 Li1 2_656 2_646 179.0(7)
O7 B3 Li1 . 2_646 60.6(5)
O6 B3 Li1 . 2_646 59.3(5)
O7 B3 Li1 2_656 1_545 60.6(5)
O7 B3 Li1 . 1_545 179.1(7)
O6 B3 Li1 . 1_545 59.3(5)
Li1 B3 Li1 2_646 1_545 118.7(9)
O7 B3 Gd3 2_656 . 60.1(5)
O7 B3 Gd3 . . 60.1(5)
O6 B3 Gd3 . . 180.000(3)
Li1 B3 Gd3 2_646 . 120.7(5)
Li1 B3 Gd3 1_545 . 120.7(5)
O7 B3 Cs1 2_656 . 108.9(2)
O7 B3 Cs1 . . 78.59(19)
O6 B3 Cs1 . . 82.8(2)
Li1 B3 Cs1 2_646 . 70.6(3)
Li1 B3 Cs1 1_545 . 101.7(4)
Gd3 B3 Cs1 . . 97.2(2)
O7 B3 Cs1 2_656 2_656 78.59(18)
O7 B3 Cs1 . 2_656 108.9(2)
O6 B3 Cs1 . 2_656 82.8(2)
Li1 B3 Cs1 2_646 2_656 101.7(4)
Li1 B3 Cs1 1_545 2_656 70.6(3)
Gd3 B3 Cs1 . 2_656 97.2(2)
Cs1 B3 Cs1 . 2_656 165.5(4)
O8 B4 O9 . . 123.9(7)
O8 B4 O10 . . 123.1(7)
O9 B4 O10 . . 112.9(9)
O9 B4 Li2 . 2_546 139.0(6)
O10 B4 Li2 . 2_546 90.4(5)
O8 B4 Gd4 . . 160.6(5)
O9 B4 Gd4 . . 55.1(5)
O10 B4 Gd4 . . 61.1(5)
Li2 B4 Gd4 2_546 . 121.1(4)
O8 B4 Cs1 . . 67.1(4)
O9 B4 Cs1 . . 68.4(4)
O10 B4 Cs1 . . 140.9(5)
Li2 B4 Cs1 2_546 . 72.4(3)
Gd4 B4 Cs1 . . 97.7(3)
O11 B5 O13 . . 123.8(7)
O11 B5 O12 . . 123.4(7)
O13 B5 O12 . . 112.7(8)
O13 B5 Li1 . 2_646 134.7(6)
O12 B5 Li1 . 2_646 93.5(5)
O11 B5 Gd5 . . 163.4(5)
O13 B5 Gd5 . . 55.1(4)
O12 B5 Gd5 . . 59.6(4)
Li1 B5 Gd5 2_646 . 123.0(4)
O11 B5 Cs1 . . 67.8(4)
O13 B5 Cs1 . . 67.9(4)
O12 B5 Cs1 . . 139.4(5)
Li1 B5 Cs1 2_646 . 68.3(3)
Gd5 B5 Cs1 . . 99.2(2)
O14 B6 O16 . . 119.6(6)
O14 B6 O15 . . 116.2(6)
O16 B6 O15 . . 124.1(7)
O14 B6 Gd3 . . 58.6(3)
O16 B6 Gd3 . . 165.9(6)
O15 B6 Gd3 . . 59.0(3)
O14 B6 Gd2 . . 72.0(4)
O16 B6 Gd2 . . 48.9(3)
O15 B6 Gd2 . . 164.3(6)
Gd3 B6 Gd2 . . 123.9(3)
O14 B6 Cs1 . . 75.0(4)
O16 B6 Cs1 . . 96.7(5)
O15 B6 Cs1 . . 99.9(5)
Gd3 B6 Cs1 . . 96.1(2)
Gd2 B6 Cs1 . . 95.2(2)
O14 B6 Cs1 . 1_565 128.9(5)
O16 B6 Cs1 . 1_565 73.6(4)
O15 B6 Cs1 . 1_565 70.0(4)
Gd3 B6 Cs1 . 1_565 96.7(2)
Gd2 B6 Cs1 . 1_565 94.4(2)
Cs1 B6 Cs1 . 1_565 156.1(3)
O11 Li1 O1 2_666 . 115.3(7)
O11 Li1 O6 2_666 1_565 138.4(7)
O1 Li1 O6 . 1_565 106.2(6)
O11 Li1 O7 2_666 2_666 103.6(7)
O1 Li1 O7 . 2_666 93.9(6)
O6 Li1 O7 1_565 2_666 71.9(5)
O11 Li1 O3 2_666 . 95.3(6)
O1 Li1 O3 . . 71.5(5)
O6 Li1 O3 1_565 . 98.4(7)
O7 Li1 O3 2_666 . 159.9(7)
O11 Li1 B3 2_666 1_565 127.1(7)
O1 Li1 B3 . 1_565 102.6(6)
O6 Li1 B3 1_565 1_565 36.1(4)
O7 Li1 B3 2_666 1_565 35.8(4)
O3 Li1 B3 . 1_565 132.3(7)
O11 Li1 B1 2_666 . 108.6(6)
O1 Li1 B1 . . 35.4(4)
O6 Li1 B1 1_565 . 105.3(6)
O7 Li1 B1 2_666 . 128.1(6)
O3 Li1 B1 . . 36.0(3)
B3 Li1 B1 1_565 . 123.3(6)
O11 Li1 B5 2_666 2_666 29.5(4)
O1 Li1 B5 . 2_666 106.0(6)
O6 Li1 B5 1_565 2_666 135.8(7)
O7 Li1 B5 2_666 2_666 76.6(5)
O3 Li1 B5 . 2_666 120.1(6)
B3 Li1 B5 1_565 2_666 107.2(6)
B1 Li1 B5 . 2_666 118.4(6)
O11 Li1 Gd1 2_666 1_565 99.0(6)
O1 Li1 Gd1 . 1_565 48.7(4)
O6 Li1 Gd1 1_565 1_565 108.1(5)
O7 Li1 Gd1 2_666 1_565 51.8(3)
O3 Li1 Gd1 . 1_565 118.9(5)
B3 Li1 Gd1 1_565 1_565 79.0(4)
B1 Li1 Gd1 . 1_565 83.4(4)
B5 Li1 Gd1 2_666 1_565 73.3(4)
O11 Li1 Gd5 2_666 2_656 48.1(4)
O1 Li1 Gd5 . 2_656 109.0(5)
O6 Li1 Gd5 1_565 2_656 118.6(6)
O7 Li1 Gd5 2_666 2_656 149.1(6)
O3 Li1 Gd5 . 2_656 51.0(3)
B3 Li1 Gd5 1_565 2_656 145.5(5)
B1 Li1 Gd5 . 2_656 79.4(4)
B5 Li1 Gd5 2_666 2_656 77.3(4)
Gd1 Li1 Gd5 1_565 2_656 133.0(4)
O11 Li1 Gd3 2_666 . 121.3(6)
O1 Li1 Gd3 . . 101.7(6)
O6 Li1 Gd3 1_565 . 46.0(4)
O7 Li1 Gd3 2_666 . 117.9(5)
O3 Li1 Gd3 . . 54.7(4)
B3 Li1 Gd3 1_565 . 82.1(5)
B1 Li1 Gd3 . . 77.0(5)
B5 Li1 Gd3 2_666 . 147.7(5)
Gd1 Li1 Gd3 1_565 . 138.9(4)
Gd5 Li1 Gd3 2_656 . 78.3(3)
O11 Li1 Cs1 2_666 2_666 64.3(4)
O1 Li1 Cs1 . 2_666 165.0(7)
O6 Li1 Cs1 1_565 2_666 75.4(3)
O7 Li1 Cs1 2_666 2_666 72.2(4)
O3 Li1 Cs1 . 2_666 123.4(5)
B3 Li1 Cs1 1_565 2_666 69.6(3)
B1 Li1 Cs1 . 2_666 159.3(6)
B5 Li1 Cs1 2_666 2_666 65.9(3)
Gd1 Li1 Cs1 1_565 2_666 116.3(4)
Gd5 Li1 Cs1 2_656 2_666 82.2(3)
Gd3 Li1 Cs1 . 2_666 90.1(3)
O8 Li2 O1 2_566 . 116.4(7)
O8 Li2 O4 2_566 1_565 130.8(6)
O1 Li2 O4 . 1_565 112.7(6)
O8 Li2 O5 2_566 1_565 105.4(6)
O1 Li2 O5 . 1_565 95.0(6)
O4 Li2 O5 1_565 1_565 73.1(5)
O8 Li2 O2 2_566 . 94.9(6)
O1 Li2 O2 . . 72.1(5)
O4 Li2 O2 1_565 . 96.6(6)
O5 Li2 O2 1_565 . 159.4(7)
O8 Li2 B2 2_566 1_565 123.2(6)
O1 Li2 B2 . 1_565 109.0(6)
O4 Li2 B2 1_565 1_565 36.4(4)
O5 Li2 B2 1_565 1_565 36.7(4)
O2 Li2 B2 . 1_565 131.5(6)
O8 Li2 B1 2_566 . 107.5(6)
O1 Li2 B1 . . 35.9(4)
O4 Li2 B1 1_565 . 109.8(6)
O5 Li2 B1 1_565 . 129.7(6)
O2 Li2 B1 . . 36.3(3)
B2 Li2 B1 1_565 . 129.2(6)
O8 Li2 B4 2_566 2_566 30.2(3)
O1 Li2 B4 . 2_566 106.8(6)
O4 Li2 B4 1_565 2_566 132.4(6)
O5 Li2 B4 1_565 2_566 78.1(5)
O2 Li2 B4 . 2_566 120.6(6)
B2 Li2 B4 1_565 2_566 105.8(6)
B1 Li2 B4 . 2_566 117.8(6)
O8 Li2 Gd1 2_566 1_565 101.7(5)
O1 Li2 Gd1 . 1_565 49.5(3)
O4 Li2 Gd1 1_565 1_565 112.6(5)
O5 Li2 Gd1 1_565 1_565 51.9(3)
O2 Li2 Gd1 . 1_565 120.7(5)
B2 Li2 Gd1 1_565 1_565 82.8(4)
B1 Li2 Gd1 . 1_565 84.7(4)
B4 Li2 Gd1 2_566 1_565 74.8(4)
O8 Li2 Gd4 2_566 2_556 46.7(3)
O1 Li2 Gd4 . 2_556 107.9(6)
O4 Li2 Gd4 1_565 2_556 113.9(5)
O5 Li2 Gd4 1_565 2_556 149.6(5)
O2 Li2 Gd4 . 2_556 50.8(3)
B2 Li2 Gd4 1_565 2_556 140.5(5)
B1 Li2 Gd4 . 2_556 77.5(4)
B4 Li2 Gd4 2_566 2_556 76.4(4)
Gd1 Li2 Gd4 1_565 2_556 133.5(4)
O8 Li2 Gd2 2_566 . 115.0(5)
O1 Li2 Gd2 . . 104.2(5)
O4 Li2 Gd2 1_565 . 46.6(4)
O5 Li2 Gd2 1_565 . 119.6(5)
O2 Li2 Gd2 . . 51.8(3)
B2 Li2 Gd2 1_565 . 83.1(4)
B1 Li2 Gd2 . . 78.0(4)
B4 Li2 Gd2 2_566 . 142.5(5)
Gd1 Li2 Gd2 1_565 . 142.6(4)
Gd4 Li2 Gd2 2_556 . 74.5(3)
O8 Li2 Cs1 2_566 2_566 59.8(3)
O1 Li2 Cs1 . 2_566 167.2(6)
O4 Li2 Cs1 1_565 2_566 73.0(3)
O5 Li2 Cs1 1_565 2_566 75.3(4)
O2 Li2 Cs1 . 2_566 119.5(5)
B2 Li2 Cs1 1_565 2_566 68.2(3)
B1 Li2 Cs1 . 2_566 154.9(6)
B4 Li2 Cs1 2_566 2_566 63.4(3)
Gd1 Li2 Cs1 1_565 2_566 118.0(4)
Gd4 Li2 Cs1 2_556 2_566 78.7(3)
Gd2 Li2 Cs1 . 2_566 88.0(3)
B1 O1 Li2 . . 88.1(6)
B1 O1 Li1 . . 88.2(6)
Li2 O1 Li1 . . 173.9(7)
B1 O1 Gd1 . 1_565 166.2(5)
Li2 O1 Gd1 . 1_565 91.0(5)
Li1 O1 Gd1 . 1_565 91.5(5)
B1 O2 Li2 . . 78.0(5)
B1 O2 Gd4 . 2_556 127.6(4)
Li2 O2 Gd4 . 2_556 86.1(4)
B1 O2 Gd1 . . 90.8(5)
Li2 O2 Gd1 . . 167.6(4)
Gd4 O2 Gd1 2_556 . 105.3(2)
B1 O2 Gd2 . . 126.5(4)
Li2 O2 Gd2 . . 86.0(4)
Gd4 O2 Gd2 2_556 . 101.29(17)
Gd1 O2 Gd2 . . 96.45(18)
B1 O3 Li1 . . 79.8(6)
B1 O3 Gd5 . 2_656 132.9(4)
Li1 O3 Gd5 . 2_656 85.3(4)
B1 O3 Gd1 . . 92.3(5)
Li1 O3 Gd1 . . 167.3(4)
Gd5 O3 Gd1 2_656 . 107.36(19)
B1 O3 Gd3 . . 118.3(4)
Li1 O3 Gd3 . . 83.9(4)
Gd5 O3 Gd3 2_656 . 103.96(17)
Gd1 O3 Gd3 . . 91.14(16)
B2 O4 Li2 . 2_546 84.3(5)
B2 O4 Li2 . 1_545 84.3(5)
Li2 O4 Li2 2_546 1_545 168.6(9)
B2 O4 Gd2 . 1_545 180.000(2)
Li2 O4 Gd2 2_546 1_545 95.7(5)
Li2 O4 Gd2 1_545 1_545 95.7(5)
B2 O4 Cs1 . . 75.18(13)
Li2 O4 Cs1 2_546 . 74.8(4)
Li2 O4 Cs1 1_545 . 102.2(4)
Gd2 O4 Cs1 1_545 . 104.82(13)
B2 O4 Cs1 . 2_556 75.19(13)
Li2 O4 Cs1 2_546 2_556 102.2(4)
Li2 O4 Cs1 1_545 2_556 74.8(3)
Gd2 O4 Cs1 1_545 2_556 104.81(13)
Cs1 O4 Cs1 . 2_556 150.4(3)
B2 O5 Li2 . 1_545 80.8(6)
B2 O5 Gd1 . . 139.4(3)
Li2 O5 Gd1 1_545 . 85.5(4)
B2 O5 Gd2 . . 92.0(5)
Li2 O5 Gd2 1_545 . 171.2(4)
Gd1 O5 Gd2 . . 103.29(19)
B2 O5 Cs1 . 2_556 71.2(2)
Li2 O5 Cs1 1_545 2_556 71.7(4)
Gd1 O5 Cs1 . 2_556 138.87(17)
Gd2 O5 Cs1 . 2_556 101.16(14)
B3 O6 Li1 . 2_646 84.6(5)
B3 O6 Li1 . 1_545 84.6(5)
Li1 O6 Li1 2_646 1_545 169.1(10)
B3 O6 Gd3 . 1_545 180.000(2)
Li1 O6 Gd3 2_646 1_545 95.4(5)
Li1 O6 Gd3 1_545 1_545 95.4(5)
B3 O6 Cs1 . . 74.35(13)
Li1 O6 Cs1 2_646 . 71.0(4)
Li1 O6 Cs1 1_545 . 105.9(4)
Gd3 O6 Cs1 1_545 . 105.65(13)
B3 O6 Cs1 . 2_656 74.35(13)
Li1 O6 Cs1 2_646 2_656 105.9(4)
Li1 O6 Cs1 1_545 2_656 71.0(4)
Gd3 O6 Cs1 1_545 2_656 105.65(13)
Cs1 O6 Cs1 . 2_656 148.7(3)
B3 O7 Li1 . 2_646 83.6(7)
B3 O7 Gd1 . 2_656 131.6(3)
Li1 O7 Gd1 2_646 2_656 86.1(4)
B3 O7 Gd3 . . 90.3(5)
Li1 O7 Gd3 2_646 . 173.9(5)
Gd1 O7 Gd3 2_656 . 98.39(18)
B3 O7 Cs1 . . 78.3(2)
Li1 O7 Cs1 2_646 . 73.2(4)
Gd1 O7 Cs1 2_656 . 142.00(18)
Gd3 O7 Cs1 . . 105.05(14)
B4 O8 Li2 . 2_546 105.4(6)
B4 O8 Gd4 . 1_545 154.9(5)
Li2 O8 Gd4 2_546 1_545 96.6(5)
B4 O8 Cs1 . . 88.9(4)
Li2 O8 Cs1 2_546 . 88.2(4)
Gd4 O8 Cs1 1_545 . 103.90(17)
B4 O9 Gd4 . 3_667 147.7(5)
B4 O9 Gd4 . . 96.9(5)
Gd4 O9 Gd4 3_667 . 107.0(2)
B4 O9 Cs1 . . 87.3(5)
Gd4 O9 Cs1 3_667 . 100.41(16)
Gd4 O9 Cs1 . . 116.95(19)
B4 O10 Gd5 . 3_667 119.8(4)
B4 O10 Gd1 . 2_556 126.6(5)
Gd5 O10 Gd1 3_667 2_556 107.16(18)
B4 O10 Gd4 . . 90.2(5)
Gd5 O10 Gd4 3_667 . 101.73(19)
Gd1 O10 Gd4 2_556 . 104.58(19)
B5 O11 Li1 . 2_646 106.8(7)
B5 O11 Gd5 . 1_545 157.8(5)
Li1 O11 Gd5 2_646 1_545 93.4(5)
B5 O11 Cs1 . . 88.4(4)
Li1 O11 Cs1 2_646 . 82.1(4)
Gd5 O11 Cs1 1_545 . 103.60(18)
B5 O12 Gd5 . 3_767 123.5(4)
B5 O12 Gd1 . 2_656 122.7(4)
Gd5 O12 Gd1 3_767 2_656 104.79(18)
B5 O12 Gd5 . . 91.1(5)
Gd5 O12 Gd5 3_767 . 105.47(19)
Gd1 O12 Gd5 2_656 . 104.85(19)
B5 O13 Gd4 . 3_667 145.3(5)
B5 O13 Gd5 . . 96.2(5)
Gd4 O13 Gd5 3_667 . 109.4(2)
B5 O13 Cs1 . . 87.7(4)
Gd4 O13 Cs1 3_667 . 98.94(15)
Gd5 O13 Cs1 . . 119.64(19)
B6 O14 Gd1 . . 169.7(4)
B6 O14 Gd3 . . 93.9(4)
Gd1 O14 Gd3 . . 95.26(17)
B6 O14 Gd2 . . 81.7(4)
Gd1 O14 Gd2 . . 88.05(15)
Gd3 O14 Gd2 . . 152.1(3)
B6 O14 Cs1 . . 80.7(4)
Gd1 O14 Cs1 . . 100.8(2)
Gd3 O14 Cs1 . . 107.41(18)
Gd2 O14 Cs1 . . 99.10(15)
B6 O15 Gd5 . . 150.6(5)
B6 O15 Gd3 . . 93.0(4)
Gd5 O15 Gd3 . . 109.51(18)
B6 O15 Cs1 . 1_565 85.3(4)
Gd5 O15 Cs1 . 1_565 102.85(18)
Gd3 O15 Cs1 . 1_565 111.43(19)
B6 O15 Cs1 . . 58.9(4)
Gd5 O15 Cs1 . . 100.28(17)
Gd3 O15 Cs1 . . 92.58(15)
Cs1 O15 Cs1 1_565 . 138.22(15)
B6 O16 Gd4 . . 144.3(5)
B6 O16 Gd2 . . 105.5(4)
Gd4 O16 Gd2 . . 107.11(19)
B6 O16 Cs1 . 1_565 82.2(4)
Gd4 O16 Cs1 . 1_565 98.27(18)
Gd2 O16 Cs1 . 1_565 112.5(2)
B6 O16 Cs1 . . 61.7(4)
Gd4 O16 Cs1 . . 99.34(18)
Gd2 O16 Cs1 . . 98.23(17)
Cs1 O16 Cs1 1_565 . 137.95(15)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Gd1 O1 1_545 2.279(6)
Gd1 O5 . 2.368(4)
Gd1 O14 . 2.373(5)
Gd1 O10 2_556 2.389(5)
Gd1 O7 2_656 2.389(4)
Gd1 O12 2_656 2.431(5)
Gd1 O3 . 2.443(5)
Gd1 O2 . 2.478(5)
Gd1 B1 . 2.860(11)
Gd1 Li2 1_545 2.999(12)
Gd1 Li1 1_545 3.033(14)
Gd1 Gd3 . 3.6274(8)
Gd2 O4 1_565 2.328(8)
Gd2 O5 . 2.377(5)
Gd2 O5 2_556 2.377(5)
Gd2 O16 2_556 2.398(5)
Gd2 O16 . 2.398(5)
Gd2 O2 . 2.511(5)
Gd2 O2 2_556 2.511(5)
Gd2 B2 . 2.786(12)
Gd2 B6 2_556 3.067(7)
Gd2 B6 . 3.067(7)
Gd3 O6 1_565 2.319(8)
Gd3 O7 . 2.403(5)
Gd3 O7 2_656 2.403(5)
Gd3 O14 . 2.535(5)
Gd3 O14 2_656 2.535(5)
Gd3 O15 2_656 2.544(5)
Gd3 O15 . 2.544(5)
Gd3 O3 2_656 2.634(5)
Gd3 O3 . 2.634(5)
Gd3 B3 . 2.772(13)
Gd3 B6 . 2.963(7)
Gd3 B6 2_656 2.963(7)
Gd4 O9 3_667 2.241(5)
Gd4 O13 3_667 2.273(5)
Gd4 O8 1_565 2.294(6)
Gd4 O16 . 2.356(6)
Gd4 O9 . 2.404(5)
Gd4 O2 2_556 2.433(5)
Gd4 O10 . 2.545(5)
Gd4 B4 . 2.908(12)
Gd4 Li2 2_556 3.132(13)
Gd4 Gd4 3_667 3.7337(10)
Gd4 Gd5 3_667 3.7958(8)
Gd5 O11 1_565 2.291(6)
Gd5 O15 . 2.309(5)
Gd5 O12 3_767 2.378(5)
Gd5 O13 . 2.379(5)
Gd5 O3 2_656 2.396(5)
Gd5 O12 . 2.489(5)
Gd5 B5 . 2.884(11)
Gd5 Li1 2_656 3.072(13)
Gd5 Gd4 3_667 3.7957(7)
Gd5 Gd1 4_666 3.8099(9)
Gd5 Gd5 3_767 3.8737(10)
Cs1 O8 . 3.069(5)
Cs1 O9 . 3.101(5)
Cs1 O11 . 3.121(5)
Cs1 O13 . 3.126(5)
Cs1 O15 1_545 3.131(5)
Cs1 O16 1_545 3.215(6)
Cs1 O14 . 3.219(6)
Cs1 B6 . 3.289(9)
Cs1 B6 1_545 3.320(9)
Cs1 B4 . 3.331(9)
Cs1 B5 . 3.370(8)
Cs1 B3 . 3.4074(19)
B1 O1 . 1.352(12)
B1 O2 . 1.391(9)
B1 O3 . 1.392(9)
B1 Li2 . 2.302(15)
B1 Li1 . 2.329(15)
B2 O4 . 1.352(14)
B2 O5 2_556 1.372(8)
B2 O5 . 1.372(8)
B2 Li2 2_546 2.265(14)
B2 Li2 1_545 2.265(14)
B2 Cs1 2_556 3.4305(18)
B3 O7 2_656 1.367(8)
B3 O7 . 1.368(8)
B3 O6 . 1.375(15)
B3 Li1 2_646 2.323(14)
B3 Li1 1_545 2.323(14)
B3 Cs1 2_656 3.4075(17)
B4 O8 . 1.355(13)
B4 O9 . 1.374(10)
B4 O10 . 1.400(10)
B4 Li2 2_546 2.597(15)
B5 O11 . 1.362(12)
B5 O13 . 1.393(10)
B5 O12 . 1.408(10)
B5 Li1 2_646 2.650(17)
B6 O14 . 1.372(9)
B6 O16 . 1.376(9)
B6 O15 . 1.393(8)
B6 Cs1 1_565 3.320(8)
Li1 O11 2_666 1.913(14)
Li1 O1 . 1.941(13)
Li1 O6 1_565 2.007(13)
Li1 O7 2_666 2.036(15)
Li1 O3 . 2.130(15)
Li1 B3 1_565 2.323(14)
Li1 B5 2_666 2.650(17)
Li1 Gd1 1_565 3.033(14)
Li1 Gd5 2_656 3.072(13)
Li1 Cs1 2_666 3.429(12)
Li2 O8 2_566 1.885(13)
Li2 O1 . 1.909(12)
Li2 O4 1_565 1.957(12)
Li2 O5 1_565 2.034(14)
Li2 O2 . 2.145(14)
Li2 B2 1_565 2.265(14)
Li2 B4 2_566 2.597(15)
Li2 Gd1 1_565 2.999(12)
Li2 Gd4 2_556 3.132(13)
Li2 Cs1 2_566 3.549(12)
O1 Gd1 1_565 2.279(6)
O2 Gd4 2_556 2.433(5)
O3 Gd5 2_656 2.396(5)
O4 Li2 2_546 1.957(12)
O4 Li2 1_545 1.957(12)
O4 Gd2 1_545 2.328(8)
O4 Cs1 2_556 3.517(2)
O5 Li2 1_545 2.034(14)
O5 Cs1 2_556 3.616(5)
O6 Li1 2_646 2.007(13)
O6 Li1 1_545 2.007(13)
O6 Gd3 1_545 2.319(8)
O6 Cs1 2_656 3.510(2)
O7 Li1 2_646 2.036(15)
O7 Gd1 2_656 2.389(4)
O8 Li2 2_546 1.885(13)
O8 Gd4 1_545 2.294(6)
O9 Gd4 3_667 2.241(5)
O10 Gd5 3_667 2.346(5)
O10 Gd1 2_556 2.389(5)
O11 Li1 2_646 1.913(14)
O11 Gd5 1_545 2.291(6)
O12 Gd5 3_767 2.378(5)
O12 Gd1 2_656 2.431(5)
O13 Gd4 3_667 2.273(5)
O15 Cs1 1_565 3.131(5)
O16 Cs1 1_565 3.215(6)
